# chapter 5: diffusion 5.1 steady-state diffusion

Post on 12-Jan-2017

239 views

Embed Size (px)

TRANSCRIPT

1

Chapter 5

Chapter 5: DiffusionDiffusion: the movement of particles in a solid from an area of high

concentration to an area of low concentration, resulting in the uniform distribution of the substance

Diffusion is process which is NOT due to the action of a force, but a result of the random movements of atoms (statistical problem)

1. Diffusivity and 2 Ficks laws

2. Atomistic mechanisms of diffusion

3. Temperature dependence and Arrenius plot

4. Industrial applications - carburized steel, - dopants in silicon

Chapter 5

5.1 Steady-State Diffusion

Recall: Solvent the majority atom type (or host atoms): Solute the element with lower concentrationSubstitutional a solid solution in which the solute atoms are replaced by soluteInterstitial solute atoms are located in gaps between host atoms

Consider diffusion of solute atoms (b) in solid state solution (AB) in direction x between two parallel atomic planes (separated by x)

if there is no changes with time in CB at these planes such diffusion condition is called steady-state diffusion

For a steady-state diffusion, flux (flow), J, of atoms is:

dxdCDJ =

J flux of atoms, atoms/(m2 s): the number of particles which pass through a unit area in a unit of time;

D diffusivity or diffusion coefficient, m2/s

dC/dx concentration gradient, atoms/m4

2

Chapter 5

Ficks first law of diffusion

For steady-state diffusion condition (no change in the system with time), the net flow of atoms is equal to the diffusivity D times the diffusion gradient dC/dxdx

dCDJ =

=

mmatoms

dxdC

smD

smatomsJ 13

2

2

Diffusivity D depends on:1. Diffusion mechanism

2. Temperature of diffusion

3. Type of crystal structure (bcc > fcc)

4. Crystal imperfections

5. Concentration of diffusing species

- sign: flux direction is from the higher to the lower concentration; i.e. it is the opposite to the concentration gradient

Chapter 5

Non-Steady-State Diffusion

In practice the concentration of solute atoms at any point in the material changes with time non-steady-state diffusion

For non-steady-state condition, diffusion coefficient, D - NOT dependent on time:

=

dxdCD

dxd

dtdC xxSecond Ficks law of diffusion:

The rate of compositional change is equal to the diffusivity times the rate of the change of the concentration gradient

2

2

xCD

dtdCx

=If D D(x), in 1D case:

+

+

= 22

2

2

2

2

zC

yC

xCD

dtdCxIn 3D case:

Change in concentration in 2 semi-infinite rods of Cu and Ni caused by diffusion, From G. Gottstein Physical Foundations of Material Science

3

Chapter 5

Non-Steady-State Diffusion (continued)

With specific initial or boundary conditions this partial differential equations can be solved to give the concentration as function of spatial position and time c(x, y, z, t)

Let us consider two rods with different concentrations c1and c2 which are joined at x=0 and both are so long that mathematically they can be considered as infinitely long

The concentration profile at t = 0 is discontinuous at x = 0:

x < 0, c = c1; x < 0, c = c2We can obtain solution of:

2

2

xCD

dtdCx

=

functionerror theasknown is ,2)( where

21

2),(

0

21212

1

2

2

=

+

=

=

z

Dtx

dezerf

Dtxerfccdeccctxc

Dtxz

2=

Chapter 5

Gas diffusion into a solid

Let us consider the case of a gas A diffusing into a solid B

Gas A Solid B

x = 0

=

Dtxerf

CCCC

oS

xs

2

CS surf. C of element in gas diffusing into the surface

Co initial uniform concentration of element in solid

x - distance from surface

D diffusivity of diffusing solute element

t time

erf mathematical function called error function

4

Chapter 5

Error function

Curve of the error function erf (z) for

Dtxz

2=

Chapter 5

Q: Consider the gas carburizing of a gear of 1018 steel (C 0.18 wt %) at 927C. Calculate the time necessary to increase the C content to 0.35 wt % at 0.40 mm below the surface of the gear. Assume the C content at the surface to be 1.15 wt % and that the nominal C content of the steel gear before carburizing is 0.18 wt %. D (C in iron) at 927C = 1.28 10-11 m2/s

5

Chapter 5

5.2 Atomistics of Solid State Diffusion

Diffusion mechanisms:1. Vacancy (substitutional) diffusion migration of atom in a lattice assisted

by the presence of vacanciesEx.: self diffusion of Cu atoms in Cu crystal2. Interstitial diffusion movement of atoms from one interstitial site to

another neighboring interstitial site without permanent displacement any of the atoms in the matrix crystal lattice

Ex.: C diffusion in BCC iron

Chapter 5

VacanciesThe simplest point defect is the vacancy (V) an atom site from which an atom is missing

Vacancies are always present; their number NV depends on temperature (T)

vacancy

kTE

V

V

eNN

=

NV - # of vacanciesN - number of lattice sitesEV energy required to form a vacancyk Boltzmann constant k = 1.38 10-23 J K-1; or 8.62 10-5 eV K-1

T absolute temperature

6

Chapter 5

Vacancy (Substitutional) Diffusion Mechanism

Substitutional (in homogeneous system - self-diffusion, in heterogeneous system solid state solutions)

Vacancies are always present at any T As T increases # of vacancies increases

diffusion rate increases Move atom A (from (1) to (2)) = move vacancy from

(2) to (1)..?

higher Tmelt stronger bonding between atoms high activation energy to move V

Chapter 5

Kirkendall effect

Marker at the diffusion interface move slightly in the opposite direction to the most rapidly moving species vacancies can move!

7

Chapter 5

Possible mechanisms of self-diffusion and their activation energy

1. Neighboring atoms exchange sites2. Ring mechanism3. Vacancy mechanism4. Direct interstitial mechanism5. Indirect interstitial mechanism

2 eV1 eV1 eV3

3.6 eV3.4 eV0.2 eV64 eV3.4 eV0.6 eV4

8 eV-8 eV1TotalFormationMigration

Chapter 5

Anisotropy Effects

From G.Gottstein Physical Foundations of Material Science

8

Chapter 5

Carbon diffusion in Fe

Jump frequency [s-1] of an atom is given by:

kTGm

e

= Usually 1013 [s-1] vibrational frequency of the atom

There is a fundamental relationship between the jump frequency and the diffusion coefficient D which is independent of mechanism and crystal structure:

66

22

==D

the jump distance of the diffusing atom =1/ the time interval between two jumps

J = JMN - JNM

32

41

32

41

= ANAM CCJ

24

2aD =

Chapter 5

Carbon diffusion in Fe

Can be derived from an atomistic considerations of the diffusion processes

J = JMN - JNM

24

2aD =

66

22

==D

C atoms are located on the octahedral interstitial sites (black circles)

Only of possible jumps of C atoms lead to flux in +x

Only 2/3 of all C atoms can jump in x direction

9

Chapter 5

5.3 Effects of T on diffusion in solids

Diffusion rate in a system will increase with temperature:

RTE

o

A

eDD

=

D diffusivity, m2/sD0- proportionality constant, m2/s, independent of TEA activation energy for diffusing species, J/molR molar gas constant R = 8.314 J mol-1 K-1; or 1.987cal mol-1K-1T absolute temperature

Chapter 5

Activation energy

A + B C + D

A (initial state) A* (final state)

only a fraction of the molecules or atoms in a system will havesufficient energy to reach E* A thermally active process is one which requires a definite amount of thermal energy to overcome an activation energy barrier and enter the reactive state

10

Chapter 5

Bolzmanns equation

kTEE

e

*

yProbabilit

On the basis of statistical analysis, Bolzmanns results showed that the probability of finding a molecule or atom at an energy level E* > the average energy E of all the molecules or atoms in a system at a particular temperature T, K, was:

where kB = 1.3810-23 J/(atom K) -Boltzmanns constant

The fraction of atoms or molecules in a system having energies > E* at a given T (where E* is much greater than the average energy of any atom or molecule:

kTE

total

eCN

n*

=

Chapter 5

Arrhenius Rate Equation

The rate of many chemical reaction as a function of temperature as follows:

RTEA

eCreactionofRate

=__

C rate constant, independent of TEA activation energyR molar gas constant R = 8.314 J mol-1 K-1; or 1.987cal mol-1K-1

T absolute temperature

11

Chapter 5

Typical Arrhenius Plot

If we rewrite in natural log plot:

RTECrate A= lnln

arate =lnbC =ln

Tx 1=

xmby +=

or in logarithmic log plot:

RTECrate A

303.2loglog 1010 =

Chapter 5

Q.: The diffusivity of Ag atoms in solid silver metal is 1.0X1017 m2/s at 500oC and 7.0x10-13 m2/s at 1000oC. Calculate the activation energy (J/mole) for the diffusion of Ag in Ag in the T range 500 to 1000oC.

12

Chapter 5

5.4 Industrial applicationsSteel Ha